Evaluation of the Shear Bond Strength of Composite Resin to Wet and Dry Enamel Using Dentin Bonding Agents Containing Various Solvents
Carounanidy Usha1, Sathyanarayanan Ramarao2, Bindu Meera John3, Praveen Rajesh4, S Swatha5
ABSTRACT Introduction: Bonding of composite resin to dentin mandates a wet substrate whereas, enamel should be dry. This may not be easily achievable in intracoronal preparations where enamel and dentin are closely placed to each other. Therefore, Dentin Bonding Agents (DBA) are recommended for enamel and dentinal bonding, where enamel is also left moist. A research question was raised if the "enamel-only" preparations will also benefit from wet enamel bonding and contemporary DBA. Aim: The aim of this study was to compare the shear bond strengths of composite resin, bonded to dry and wet enamel using fifth generation DBA (etch and rinse system) containing various solvents such as ethanol/water, acetone and ethanol. Materials and Methods: The crowns of 120 maxillary premolars were split into buccal and lingual halves. They were randomly
allocated into four groups of DBA: Group 1-water/ethanol based, Group 2-acetone based, Group 3-ethanol based, Group 4-universal bonding agent (control group). The buccal halves and lingual halves were bonded using the wet bonding and dry bonding technique respectively. After application of the DBAs and composite resin build up, shear bond strength testing was done. Results: Group 1 (ethanol/water based ESPE 3M, Adper Single Bond) showed highest bond strength of (23.15 MPa) in dry enamel. Group 2 (acetone based Denstply, Prime and Bond NT, showed equal bond strength in wet and dry enamel condition (18.87 MPa and 18.02 MPa respectively). Conclusion: Dry enamel bonding and ethanol/water based etch and rinse DBA can be recommended for "enamel-only" tooth preparations.
Keywords: Dry enamel bonding, Enamel-only, Wet bonding
INTRODUCTION Predictable bond strength of 20-25 MPa can be achieved in bonding composite resin to acid-etched enamel surface . Contamination of the surface lowers the bond strength by 20% to 100%; thus, moisture control is a mandatory part of enamel bonding . Unlike enamel, dentin as a bonding substrate posed numerous challenges with regards to its mineral and water content . Complete drying of the dentin resulted in poor bond strength with composite resin which led to the ‘Wet bonding concept’ where the dentin is intentionally left moist . Generations of DBA evolved to achieve a predictable bonding to dentin . The fifth generation DBAs are also known as etch and rinse systems, use the total etch and wet bonding concepts. Studies have shown that they provide better bonding than even the latest generation DBAs [6-9]. In intracoronal cavity preparations, where the enamel and dentin are closely placed to each other, it is clinically challenging to dry the enamel but keep only the dentin moist. Therefore, while using the contemporary DBAs, it is recommended that enamel is also kept moist. The clinical outcome of such intracoronal restorations might be majorly influenced by the bonding ability of larger surface of dentin than by the enamel’s bonding. But some of the restorative procedures that involve only the enamel, such as pit and fissure sealant or diastema closure or direct veneering procedures, rely solely on enamel adhesion. Adopting the same wet bonding concept in these "enamel-only" preparations, eliminates the visualization of frosty white appearance after etching. This appearance has been the reliable indicator for proper etching of enamel. Consequently, there appears a lack of clinical validation of micromechanical retention that is generated from the enamel microporosities and also on thorough removal of the moisture from enamel crystallites. Journal of Clinical and Diagnostic Research. 2017 Jan, Vol-11(1): ZC41-ZC44
Therefore, it becomes mandatory to assess and support this wet enamel bonding concept with robust scientific evidence. Current literature shows comparisons between the self-etch systems and etch and rinse systems on the moist enamel [10-13], and few studies have compared the influence of solvents in etch and rinse systems on moist enamel [14-17]. Thus, the aim of this study was to compare the shear bond strength of composite resin, bonded to enamel when dry and when moist, using fifth generation DBA (one bottle-two step etch and rinse system) containing various solvents such as ethanol/water, acetone and ethanol.
MATERIALS AND METHODS Approval for this in vitro study was obtained from the Institutional Ethical Committee of Indira Gandhi Institute of Dental Sciences, Pondicherry, India. Patients in the age group of 18-25 years, who were undergoing maxillary premolar extraction for orthodontic reasons, were selected from the outpatient department of this institute. Informed consent was obtained from them. The extracted teeth were examined thoroughly. Teeth showing carious, noncarious, developmental defects and craze lines/fractures were excluded. A total of 120 premolars were selected, external debris was removed using ultrasonic scaler. The roots were removed and the crowns were split longitudinally in mesiodistal direction as buccal and lingual halves using diamond disc under running water mounted on a slow speed hand piece. The samples were randomly divided into four groups of 30 pairs each, using a simple lot method. An unfilled resin was used as the control. The following fifth generation DBA (one bottle-two step etch and rinse system) were used: Group 1: (G1) used the water/ethanol 41
Carounanidy Usha et al., Shear Bond Strength of Composite Resin to Wet and Dry Enamel
based DBA. (Water- 5%, Ethanol- 25%) (3M ESPE-Adper Single Bond-USA) Group 2: (G2) used the acetone based DBA. (Dentsply Prime and Bond NT-Australia) Group 3: (G3) used the ethanol based DBA. (Ethanol- 25%) (IvoclarTetric N bond-Liechtenstein) The details of the DBA used in the study are shown in [Table/ Fig-1]. The samples were embedded individually in acrylic resin blocks of (1x5 cm) exposing the buccal and lingual surface. The surfaces were flattened with silica carbide abrasives under running water to create flat surface of enamel. The smear layer that might be created on the surface of the enamel after abrasion were removed after acid etching as all the adhesives tested in this study were etch and rinse adhesive systems. Adhesive tape with a circular window of 3 mm was cut using a punch holder. These cut adhesive tapes were pasted on the flat enamel surface exposing 3 mm diameter. Among the pairs, the buccal surface was used for wet bonding method and the lingual surface was used for dry bonding method. Acid etching was done with 37% phosphoric acid (N-etch-Ivoclar Vivadent) for 15 seconds. Surface was air dried thoroughly till a frosty white appearance was seen, for dry bonding. In wet bonding method, after the acid was rinsed off, the enamel was left moist and glistening. The surface was dried with gentle stream of oil-free compressed air for five seconds, from 10 cm distance, at 45° angle. For all the four groups the DBA were applied using applicator tip as per the manufacturer’s instruction. A transparent plastic tube of 3x2 mm dimension was placed perpendicularly over the enamel surface. The bonding agent was cured along with the transparent tube. Composite resin was condensed using a teflon coated plastic instrument into these tubes. A cover slip was placed on the top and the resin was polymerized in bulk with LED curing unit (L1330232, Gulin wood pecker, London, UK) with 800 mW/cm2 intensity for 40 seconds. The composite was over cured as literature shows better microhardness which would help in shear bond strength testing without any adverse effects of over curing . Trade Name
ESPE Adper Single Bond
3M ESPE, USA
Prime and Bond NT
Tetric N Bond
Lot No 51202
Bis-GMA, HEMA, dimethacrylates, methacrylated poly- alkenoic acid, copolymer, initiators, water and ethanol
UDMA, PENTA, R5-62-1 resin, T-resin, D-resin, butylatedhydroxitoluene, EDMAB, cetylaminehydrofluoride, initia- tor, stabilizers, acetone and fumed silica nanofillers BIS-GMA, UDMA, dimethacrylates, HEAM, phosphonic acid acrylates, Sio2, ethanol
[Table/Fig-1]: Dentin bonding materials used.
Testing of the shear bond strength was done at Bangalore Composite Technology Park, Bengaluru, Karnataka, India. Samples were subjected to shear bond strength test using universal testing machine (LR50K-LLOYD) at a cross head speed of 0.5 mm per minute until failure occurred. The point at which failure occurred was recorded in Newton and converted into MPa. The obtained data were tabulated.
Statistical analysis Statistical analyses were done using Graphpad InStat 3.ink. Student t-tests were done to study the effects of wet or dry enamel for each material. One-way analysis of variance (ANOVA) followed by posthoc Tukey–Kramer multiple comparison test was used to study the effectiveness of dry and wet enamel condition for all groups.
RESULTS Intra Group Analysis [Table/Fig-2] Group 1, ethanol/water based DBA 3M ESPE-Adper Single Bond, showed mean shear bond strength of 23.15±1.72 MPa in dry enamel substrate followed by Group 2, acetone based DBA, Prime and Bond NT, and Group 3, ethanol based DBA, Tetric N Bond that showed 18.02±0.75 and 14.85±0.53 MPa respectively. In wet enamel bonding, acetone based DBA showed the highest mean shear bond strength of 18.87±0.78 MPa. This was followed by ethanol based DBA that showed bond strength values of 15.16±0.50 MPa. The acetone based and the ethanol based DBA showed better bond strength values in wet enamel substrate than in dry. However, this difference was not statistically significant. The water/ethanol based DBA showed better bond strength in dry enamel than in wet enamel. The difference between dry and wet is statistically significant (p